High-pressure- and low-temperature-induced changes in [(CH3)2NH(CH2)2NH3][SbCl5].
Bujak, Maciej; Angel, Ross J.; The journal of physical chemistry. B 110 (2006) 10322–10331; doi:10.1021/jp060652v

data_1505741
_publ_section_title
;
 High-pressure- and low-temperature-induced changes in
 [(CH3)2NH(CH2)2NH3][SbCl5].
;
_journal_issue                   21
_journal_name_full               'The journal of physical chemistry. B'
_journal_page_first              10322
_journal_page_last               10331
_journal_paper_doi               10.1021/jp060652v
_journal_volume                  110
_journal_year                    2006
_chemical_formula_moiety         '2(C4 H14 N2), Cl6 Sb, Cl4 Sb'
_chemical_formula_sum            'C8 H28 Cl10 N4 Sb2'
_chemical_formula_weight         778.34
_chemical_name_common
; 
  N,N-Dimethylethylenediammonium Pentachloroantimonate(III)  
;
_chemical_name_systematic
; 
  N,N-Dimethylethylenediammonium Pentachloroantimonate(III)  
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     Patterson
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.205(7)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   24.3137(13)
_cell_length_b                   9.9272(5)
_cell_length_c                   9.9246(4)
_cell_measurement_pressure       2000000
_cell_measurement_reflns_used    29
_cell_measurement_temperature    297(2)
_cell_measurement_theta_max      12.6
_cell_measurement_theta_min      4.3
_cell_volume                     2288.3(2)
_computing_cell_refinement
;
 Single software; Angel, R. J.; Downs, R. T.; Finger, L. W. High-Pressure and 
 High-Temperature Crystal Chemistry; edited by R. M. Hazen and R. T. Downs, 
 pp. 559 - 596. The Mineralogical  Society of America: Washington DC, 2000 
;
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2004)'
_computing_data_reduction
; 
 CrysAlis RED (Oxford Diffraction, 2004); AVERAGE v2.2 (R. J. Angel, 2003), 
 www. crystal.vt.edu 
;
_computing_molecular_graphics    'Bruker SHELXTL NT (Sheldrick, 2001)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_environment      'Diamond-anvil cell, N~2~ pressure medium'
_diffrn_ambient_pressure         2000000
_diffrn_ambient_temperature      297(2)
_diffrn_measured_fraction_theta_full 0.359
_diffrn_measured_fraction_theta_max 0.359
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur-1'
_diffrn_measurement_method       \w-scans
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.061
_diffrn_reflns_av_sigmaI/netI    0.8853
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       0
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            1447
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.97
_exptl_absorpt_coefficient_mu    3.532
_exptl_absorpt_correction_T_max  0.7653
_exptl_absorpt_correction_T_min  0.4844
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
  Correction for absorption affects of the diamond anvil cell
  and the sample were made using ABSORB 6.0;  
  R. J. Angel, J. Appl. Cryst. (2004) 37, 486
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.259
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1504
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.614
_refine_diff_density_min         -0.424
_refine_diff_density_rms         0.095
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     217
_refine_ls_number_reflns         1447
_refine_ls_number_restraints     224
_refine_ls_restrained_S_all      1.022
_refine_ls_R_factor_all          0.1583
_refine_ls_R_factor_gt           0.0566
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0252P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0800
_refine_ls_wR_factor_ref         0.0937
_reflns_number_gt                902
_reflns_number_total             1447
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            jp060652vsi20060131_042319.cif
_cod_data_source_block           2.00GPa
_cod_depositor_comments
;
The following automatic conversions were performed:
'_atom_site_symetry_multiplicity' tag replaced with
'_atom_site_symmetry_multiplicity'.

Automatic conversion script
Id: cif_correct_tags 1440 2010-10-19 06:21:57Z saulius 
;
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               1505741